#------------------------------------------------------------------------------
#$Date: 2016-03-23 20:26:43 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179412 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/09/4330904.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4330904
loop_
_publ_author_name
'Wenlong Yin'
'Wendong Wang'
'Lei Bai'
'Kai Feng'
'Youguo Shi'
'Wenyu Hao'
'Jiyong Yao'
'Yicheng Wu'
_publ_contact_author_address
;
Center for Crystal Research and Development, 
Technical Institute of Physics and Chemistry, Chinese Academy of Sciences, 
Beijing 100190, P.R. China
;
_publ_contact_author_email       jyao@mail.ipc.ac.cn
_publ_contact_author_name        'Jiyong Yao'
_publ_section_title
;
 Syntheses, Structures, Physical Properties, and Electronic Structures of
 Ba2MLnTe5 (M = Ga and Ln = Sm, Gd, Dy, Er, Y; M = In and Ln = Ce, Nd, Sm,
 Gd, Dy, Er, Y)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11736
_journal_page_last               11744
_journal_paper_doi               10.1021/ic301655e
_journal_volume                  51
_journal_year                    2012
_chemical_formula_sum            'Ba2 Dy In Te5'
_chemical_formula_weight         1190.00
_space_group_IT_number           36
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'C 2c -2'
_symmetry_space_group_name_H-M   'C m c 21'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2012-07-24 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   4.5198(9)
_cell_length_b                   20.065(4)
_cell_length_c                   14.089(3)
_cell_measurement_reflns_used    2642
_cell_measurement_temperature    153(2)
_cell_measurement_theta_max      30.0182
_cell_measurement_theta_min      2.0299
_cell_volume                     1277.7(5)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  Diamond
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      153(2)
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Rigaku AFC10 diffractometer'
_diffrn_measurement_method       dtprofit.ref
_diffrn_radiation_monochromator  'Graphite Monochromator'
_diffrn_radiation_source         'Rotating Anode'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0468
_diffrn_reflns_av_sigmaI/netI    0.0688
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            4696
_diffrn_reflns_theta_full        30.05
_diffrn_reflns_theta_max         30.05
_diffrn_reflns_theta_min         2.89
_exptl_absorpt_coefficient_mu    24.772
_exptl_absorpt_correction_T_max  0.180
_exptl_absorpt_correction_T_min  0.040
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'face indexed'
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    6.186
_exptl_crystal_description       Prism
_exptl_crystal_F_000             1948
_exptl_crystal_size_max          0.2860
_exptl_crystal_size_mid          0.1150
_exptl_crystal_size_min          0.0700
_refine_diff_density_max         1.779
_refine_diff_density_min         -3.207
_refine_diff_density_rms         0.447
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.04(2)
_refine_ls_extinction_coef       0.00078(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.999
_refine_ls_matrix_type           full
_refine_ls_number_parameters     56
_refine_ls_number_reflns         1993
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      0.999
_refine_ls_R_factor_all          0.0320
_refine_ls_R_factor_gt           0.0298
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0100P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0596
_refine_ls_wR_factor_ref         0.0601
_reflns_number_gt                1873
_reflns_number_total             1993
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic301655e_si_002_11.cif
_cod_data_source_block           Ba2InDyTe5
_cod_original_cell_volume        1277.7(4)
_cod_database_code               4330904
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'x, -y, z+1/2'
'-x, y, z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ba1 Ba 1.0000 0.86955(4) 0.68437(6) 0.00624(18) Uani 1 2 d S
Ba2 Ba 1.0000 0.88096(5) 0.31746(5) 0.00605(18) Uani 1 2 d S
In In 1.0000 0.55594(6) 0.56569(7) 0.0068(2) Uani 1 2 d S
Dy Dy 1.0000 0.79091(4) 0.98195(5) 0.00633(14) Uani 1 2 d S
Te1 Te 1.0000 0.64319(5) 0.99892(7) 0.00582(19) Uani 1 2 d S
Te2 Te 1.0000 0.70780(5) 0.33825(6) 0.0056(2) Uani 1 2 d S
Te3 Te 1.0000 0.69016(5) 0.63536(6) 0.0058(2) Uani 1 2 d S
Te4 Te 1.0000 0.49591(5) 0.73782(7) 0.00583(18) Uani 1 2 d S
Te5 Te 1.0000 0.95090(5) 0.94835(7) 0.0062(2) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
In In -0.7276 1.3100 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Te1 Ba1 Te1 81.45(3) 6_664 6_764
Te1 Ba1 Te4 129.85(3) 6_664 5
Te1 Ba1 Te4 78.07(2) 6_764 5
Te1 Ba1 Te4 78.07(2) 6_664 5_455
Te1 Ba1 Te4 129.85(3) 6_764 5_455
Te4 Ba1 Te4 81.02(3) 5 5_455
Te1 Ba1 Te2 148.97(4) 6_664 6_765
Te1 Ba1 Te2 90.76(2) 6_764 6_765
Te4 Ba1 Te2 76.66(3) 5 6_765
Te4 Ba1 Te2 127.55(3) 5_455 6_765
Te1 Ba1 Te2 90.76(2) 6_664 6_665
Te1 Ba1 Te2 148.97(4) 6_764 6_665
Te4 Ba1 Te2 127.55(3) 5 6_665
Te4 Ba1 Te2 76.66(3) 5_455 6_665
Te2 Ba1 Te2 80.57(3) 6_765 6_665
Te1 Ba1 Te3 77.61(2) 6_664 .
Te1 Ba1 Te3 77.61(2) 6_764 .
Te4 Ba1 Te3 139.159(17) 5 .
Te4 Ba1 Te3 139.159(17) 5_455 .
Te2 Ba1 Te3 71.38(3) 6_765 .
Te2 Ba1 Te3 71.38(3) 6_665 .
Te1 Ba1 Ba1 130.722(16) 6_664 1_655
Te1 Ba1 Ba1 49.277(16) 6_764 1_655
Te4 Ba1 Ba1 49.488(16) 5 1_655
Te4 Ba1 Ba1 130.513(16) 5_455 1_655
Te2 Ba1 Ba1 49.714(16) 6_765 1_655
Te2 Ba1 Ba1 130.286(16) 6_665 1_655
Te3 Ba1 Ba1 90.0 . 1_655
Te1 Ba1 Ba1 49.277(16) 6_664 1_455
Te1 Ba1 Ba1 130.722(16) 6_764 1_455
Te4 Ba1 Ba1 130.513(16) 5 1_455
Te4 Ba1 Ba1 49.488(16) 5_455 1_455
Te2 Ba1 Ba1 130.286(16) 6_765 1_455
Te2 Ba1 Ba1 49.714(16) 6_665 1_455
Te3 Ba1 Ba1 90.0 . 1_455
Ba1 Ba1 Ba1 180.0 1_655 1_455
Te1 Ba2 Te1 81.95(3) 6_764 6_664
Te1 Ba2 Te2 78.32(2) 6_764 .
Te1 Ba2 Te2 78.32(2) 6_664 .
Te1 Ba2 Te4 85.09(2) 6_764 6_764
Te1 Ba2 Te4 138.91(3) 6_664 6_764
Te2 Ba2 Te4 136.37(2) . 6_764
Te1 Ba2 Te4 138.91(3) 6_764 6_664
Te1 Ba2 Te4 85.09(2) 6_664 6_664
Te2 Ba2 Te4 136.37(2) . 6_664
Te4 Ba2 Te4 79.57(3) 6_764 6_664
Te1 Ba2 Te3 149.26(4) 6_764 6_664
Te1 Ba2 Te3 93.42(2) 6_664 6_664
Te2 Ba2 Te3 70.99(3) . 6_664
Te4 Ba2 Te3 116.09(3) 6_764 6_664
Te4 Ba2 Te3 70.07(3) 6_664 6_664
Te1 Ba2 Te3 93.42(2) 6_764 6_764
Te1 Ba2 Te3 149.26(4) 6_664 6_764
Te2 Ba2 Te3 70.99(3) . 6_764
Te4 Ba2 Te3 70.07(3) 6_764 6_764
Te4 Ba2 Te3 116.09(3) 6_664 6_764
Te3 Ba2 Te3 75.18(3) 6_664 6_764
Te1 Ba2 Te5 76.56(2) 6_764 2_774
Te1 Ba2 Te5 76.56(2) 6_664 2_774
Te2 Ba2 Te5 146.52(3) . 2_774
Te4 Ba2 Te5 62.52(3) 6_764 2_774
Te4 Ba2 Te5 62.52(3) 6_664 2_774
Te3 Ba2 Te5 132.08(2) 6_664 2_774
Te3 Ba2 Te5 132.08(2) 6_764 2_774
Te1 Ba2 Ba2 49.027(15) 6_764 1_655
Te1 Ba2 Ba2 130.974(15) 6_664 1_655
Te2 Ba2 Ba2 90.0 . 1_655
Te4 Ba2 Ba2 50.213(16) 6_764 1_655
Te4 Ba2 Ba2 129.787(16) 6_664 1_655
Te3 Ba2 Ba2 127.587(14) 6_664 1_655
Te3 Ba2 Ba2 52.411(14) 6_764 1_655
Te5 Ba2 Ba2 90.0 2_774 1_655
Te1 Ba2 Ba2 130.974(15) 6_764 1_455
Te1 Ba2 Ba2 49.027(15) 6_664 1_455
Te2 Ba2 Ba2 90.0 . 1_455
Te4 Ba2 Ba2 129.787(16) 6_764 1_455
Te4 Ba2 Ba2 50.213(16) 6_664 1_455
Te3 Ba2 Ba2 52.411(14) 6_664 1_455
Te3 Ba2 Ba2 127.587(14) 6_764 1_455
Te5 Ba2 Ba2 90.0 2_774 1_455
Ba2 Ba2 Ba2 180.0 1_655 1_455
Te4 In Te5 120.42(3) . 6_664
Te4 In Te5 120.42(3) . 6_764
Te5 In Te5 107.44(5) 6_664 6_764
Te4 In Te3 96.39(4) . .
Te5 In Te3 104.36(4) 6_664 .
Te5 In Te3 104.36(4) 6_764 .
Te1 Dy Te2 93.56(3) . 6_665
Te1 Dy Te2 93.56(3) . 6_765
Te2 Dy Te2 96.28(3) 6_665 6_765
Te1 Dy Te3 93.73(3) . 6_765
Te2 Dy Te3 172.36(3) 6_665 6_765
Te2 Dy Te3 85.56(2) 6_765 6_765
Te1 Dy Te3 93.73(3) . 6_665
Te2 Dy Te3 85.56(2) 6_665 6_665
Te2 Dy Te3 172.36(3) 6_765 6_665
Te3 Dy Te3 91.68(3) 6_765 6_665
Te1 Dy Te5 176.23(4) . .
Te2 Dy Te5 83.93(3) 6_665 .
Te2 Dy Te5 83.93(3) 6_765 .
Te3 Dy Te5 88.90(3) 6_765 .
Te3 Dy Te5 88.90(3) 6_665 .
Dy Te1 Ba2 94.62(3) . 6_665
Dy Te1 Ba2 94.62(3) . 6_765
Ba2 Te1 Ba2 81.95(3) 6_665 6_765
Dy Te1 Ba1 97.71(3) . 6_765
Ba2 Te1 Ba1 167.67(3) 6_665 6_765
Ba2 Te1 Ba1 96.97(2) 6_765 6_765
Dy Te1 Ba1 97.71(3) . 6_665
Ba2 Te1 Ba1 96.97(2) 6_665 6_665
Ba2 Te1 Ba1 167.67(3) 6_765 6_665
Ba1 Te1 Ba1 81.45(3) 6_765 6_665
Dy Te2 Dy 96.28(3) 6_764 6_664
Dy Te2 Ba2 92.72(3) 6_764 .
Dy Te2 Ba2 92.72(3) 6_664 .
Dy Te2 Ba1 154.06(4) 6_764 6_664
Dy Te2 Ba1 86.34(2) 6_664 6_664
Ba2 Te2 Ba1 112.98(3) . 6_664
Dy Te2 Ba1 86.34(2) 6_764 6_764
Dy Te2 Ba1 154.06(4) 6_664 6_764
Ba2 Te2 Ba1 112.98(3) . 6_764
Ba1 Te2 Ba1 80.57(3) 6_664 6_764
In Te3 Dy 83.01(3) . 6_664
In Te3 Dy 83.01(3) . 6_764
Dy Te3 Dy 91.68(3) 6_664 6_764
In Te3 Ba1 170.83(4) . .
Dy Te3 Ba1 90.62(3) 6_664 .
Dy Te3 Ba1 90.62(3) 6_764 .
In Te3 Ba2 82.83(3) . 6_765
Dy Te3 Ba2 163.58(4) 6_664 6_765
Dy Te3 Ba2 94.82(2) 6_764 6_765
Ba1 Te3 Ba2 104.35(3) . 6_765
In Te3 Ba2 82.83(3) . 6_665
Dy Te3 Ba2 94.82(2) 6_664 6_665
Dy Te3 Ba2 163.58(4) 6_764 6_665
Ba1 Te3 Ba2 104.35(3) . 6_665
Ba2 Te3 Ba2 75.18(3) 6_765 6_665
In Te4 Ba1 97.49(3) . 5_445
In Te4 Ba1 97.49(3) . 5_545
Ba1 Te4 Ba1 81.02(3) 5_445 5_545
In Te4 Ba2 88.47(3) . 6_765
Ba1 Te4 Ba2 173.93(4) 5_445 6_765
Ba1 Te4 Ba2 99.38(2) 5_545 6_765
In Te4 Ba2 88.47(3) . 6_665
Ba1 Te4 Ba2 99.38(2) 5_445 6_665
Ba1 Te4 Ba2 173.93(4) 5_545 6_665
Ba2 Te4 Ba2 79.58(3) 6_765 6_665
In Te5 In 107.44(5) 6_765 6_665
In Te5 Dy 82.27(3) 6_765 .
In Te5 Dy 82.27(3) 6_665 .
In Te5 Ba2 109.01(3) 6_765 2_775
In Te5 Ba2 109.01(3) 6_665 2_775
Dy Te5 Ba2 159.73(4) . 2_775
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 Te1 3.4640(11) 6_664
Ba1 Te1 3.4640(11) 6_764
Ba1 Te4 3.4788(11) 5
Ba1 Te4 3.4788(11) 5_455
Ba1 Te2 3.4951(11) 6_765
Ba1 Te2 3.4951(11) 6_665
Ba1 Te3 3.6650(15) .
Ba1 Ba1 4.5198(9) 1_655
Ba1 Ba1 4.5198(9) 1_455
Ba2 Te1 3.4465(10) 6_764
Ba2 Te1 3.4465(10) 6_664
Ba2 Te2 3.4868(15) .
Ba2 Te4 3.5314(12) 6_764
Ba2 Te4 3.5314(12) 6_664
Ba2 Te3 3.7049(11) 6_664
Ba2 Te3 3.7049(11) 6_764
Ba2 Te5 3.8450(15) 2_774
Ba2 Ba2 4.5198(9) 1_655
Ba2 Ba2 4.5198(9) 1_455
In Te4 2.7078(15) .
In Te5 2.8034(9) 6_664
In Te5 2.8034(9) 6_764
In Te3 2.8665(16) .
Dy Te1 2.9736(13) .
Dy Te2 3.0343(8) 6_665
Dy Te2 3.0343(8) 6_765
Dy Te3 3.1501(9) 6_765
Dy Te3 3.1501(9) 6_665
Dy Te5 3.2449(14) .
Te1 Ba2 3.4465(10) 6_665
Te1 Ba2 3.4465(10) 6_765
Te1 Ba1 3.4640(11) 6_765
Te1 Ba1 3.4640(11) 6_665
Te2 Dy 3.0343(8) 6_764
Te2 Dy 3.0343(8) 6_664
Te2 Ba1 3.4951(11) 6_664
Te2 Ba1 3.4951(11) 6_764
Te3 Dy 3.1501(9) 6_664
Te3 Dy 3.1501(9) 6_764
Te3 Ba2 3.7048(11) 6_765
Te3 Ba2 3.7048(11) 6_665
Te4 Ba1 3.4789(11) 5_445
Te4 Ba1 3.4789(11) 5_545
Te4 Ba2 3.5314(12) 6_765
Te4 Ba2 3.5314(11) 6_665
Te5 In 2.8034(9) 6_765
Te5 In 2.8034(9) 6_665
Te5 Ba2 3.8450(15) 2_775
